FEEDSTOCK RECYCLING OF AGRICULTURE PLASTIC FILM
WASTES BY CATALYTIC CRACKING
D.P. Serrano1*, J. Aguado1, J. M. Escola1, E. Garagorri2, J. M. Rodríguez1, L. Morselli3, G.
Palazzi3 and R. Orsi3
Published on: Appl. Catal. B: 49(4) 257 – 265 (2004)
Línea de investigación: Reciclado químico de plásticos
Temática madroño: Medio Ambiente
1Department of Chemical, Environmental and Materials Technology,
Rey Juan Carlos University, Escuela Superior de Ciencias Experimentales y Tecnología
(ESCET), 28933, Móstoles (Spain)
2Chemical Engineering Department, Complutense University, 28040, Madrid (Spain)
3Faculty of Industrial Chemistry, University of Bologna, 40136 Bologna (Italy)
Tel: +34 91 664 74 50
Fax: +34 91 664 74 90
Feedstock recycling by catalytic cracking of a real plastic film waste from Almeria
greenhouses (Spain) towards valuable hydrocarbon mixtures has been studied over several acid
catalysts. The plastic film waste was mostly made up of ambient degraded low-density
polyethylene (LDPE) and ethylene-vinyl acetate copolymer (EVA), the vinyl acetate content being
around 4 wt %. Nanocrystalline HZSM-5 zeolite (crystal size 60 nm) was the only catalyst
capable of degrading completely the refuse at 420ºC despite using a very small amount of
catalyst (plastic / catalyst mass ratio of 50). However, mesoporous catalysts (SBA-15 and
Al-MCM-41), unlike it occurred with virgin LDPE, showed fairly close conversions to that of thermal
cracking. Nanocrystalline HZSM-5 zeolite led to 60 wt % selectivity towards C1 - C5 hydrocarbons,
mostly valuable C3 - C5 olefins, what would improve the profitability of a future industrial recycling
process. The remarkable performance of nanocrystalline HZSM-5 zeolite was ascribed to its high
content of strong external acid sites due to its nanometer dimension, which are very active for the
cracking of bulky macromolecules. Hence, nanocrystalline HZSM-5 can be regarded as a
promising catalyst for a feasible feedstock recycling process by catalytic cracking.
Plastic wastes have become a subject of increasing worldwide environmental concern.
According to 2000 data , the total plastic consumption in Western Europe increased to 35.8
million tonnes (Mt). The plastic wastes collected this same year amounted to 18.8 Mt, the great
majority ending up their lifetime as a part of the municipal solid waste stream (MSW). In 1994, the
European Union, aware of this problem, launched the 94/62/CE directive on waste packaging that
established minimum rates of recycling per material (15 %). Since then, the percentages of
recycling and energy recovery have increased to 12.6 % and 20.2 % respectively, but the
preferred management strategies of plastic wastes is still landfilling (64 %).
The development of recycling procedures for polyolefins such as low-density
polyethylene (LDPE), high-density polyethylene (HDPE) and polypropylene (PP), is highly
encouraged since they account for roughly 60 % of the total plastic wastes . In practice, these
polyolefin refuse can be recycled either mechanically towards a new plastic with similar / lower
applications, or chemically to obtaining chemical raw materials or fuels. However, mechanical
recycling should be regarded as an intermediate procedure due to their inherent bounds
(progressive loss of plastic properties through melting, saturation of potential end-markets, etc.)
. Thus, sooner or latter, mechanically recycled plastics should be treated by other procedures
such as feedstock recycling, energy recovery or landfilling.
Feedstock recycling is becoming an increasingly promising alternative . Several
polyolefin feedstock recycling procedures have been proposed based on gasification [5,6],
hydrogenation , thermal pyrolysis , catalytic cracking , and also recently, its usage as coke
hydrocarbons mixtures with controlled compositions useful either as fuels or even raw chemicals,
is a matter of increasing research [10 - 16]. In this regard, conventional cracking catalysts
(silica-alumina, zeolites, FCC catalysts) [10, 13] as well as new ones with a high share of fully
accessible acid sites over its huge external surface (nanocrystalline ZSM-5) or inside the
mesopores (AlMCM-41) have been tested . The latter have exhibited a remarkable
performance since they were capable of surpassing the steric hindrances posed by the bulky
nature of the polymer macromolecules. In addition, selectivity can be tailored by a judicious
choice of both the acid properties and porous structure of the catalysts .
However, the great majority of catalytic cracking studies have been carried out with virgin
plastics so there are some reasonable doubts about their behavior in case of using real plastic
wastes. The presence of different polymers in the real plastic waste makeup, additives, fillers,
pollutants, dirt and also the unavoidable degradation of the polymer main chain caused by their
usage in the environment (mostly UV and air exposure) is supposed to influence heavily both the
activity and selectivity of the catalysts. Accordingly, the present work is aimed at studying the
performance of several acid catalysts (nanocrystalline HZSM-5, Al-MCM-41, Al-SBA-15, and
TiAl-Beta zeolite) for the cracking of a real agriculture film waste coming from Almeria greenhouses
(Spain). Some of these catalysts showed previously a high activity in the cracking of a
polyethylene-rich polyolefin mixture . The experimental results reported in this work point out
that nanocrystalline HZSM-5 exhibits a highly remarkable performance for the cracking of these
kind of residues whereas mesoporous materials (Al-MCM-41, Al-SBA-15), unlike it occurred in
2. Experimental Section
2A. Catalysts. The catalysts used in the present research were Al-SBA-15, Al-MCM-41 and both
nanometer size HZSM-5 (n-HZSM-5) and TiAl-Beta zeolites. All these catalysts were synthesized
in our laboratory according to procedures published in literature [17-19]. The prepared materials
were characterized by means of a number of conventional techniques. XRF fluorescence
analyses were performed in a Philips PW 1404 spectrometer. XRD measurements were taken in
a Philips X´PERT MPD diffractometer using Cu K radiation with step size and a counting time of
0.02º and 10 s, respectively. Nitrogen adsorption isotherms were obtained in a Micromeritics
ASAP 2010 sorptometer recording both adsorption and desorption branches of the isotherms.
Previously, the samples were outgassed at 250º C under vacuum for 5 h. The total surface area
values were obtained by application of the BET equation whereas the external surface of the
samples were calculated by the t-plot procedure. The pore size distributions were determined by
applicacion of the Barrett-Joyner-Halenda method (BJH) to the adsorption branch of the isotherm
assuming cylindrical pore geometry. NH3 TPD measurements were carried out in a Micromeritics
2910 (TPD/TPR) equipment. Previously, the samples were outgassed under a He flow (50 Nml
min-1) by heating with a rate of 15ºC min-1 up to 550ºC. An ammonia flow of 35 Nml min-1 was
passed through the sample for 30 min at 180ºC. The physisorbed ammonia was removed by
flowing He (180ºC, 90 min) and subsequently, the chemically adsorbed ammonia was desorbed
by increasing the temperature up to 550ºC (heating rate 15ºC min-1), measuring its
concentration by a thermal conductivity detector. 27Al-MAS-NMR spectra of the calcined catalysts
were obtained at 104.26 MHz using a Bruker MSL-400 spectrometer equipped with a Fourier
Transform unit with [Al(H2O)6+3] as external standard. All the measurements were carried out at
successive accumulations. TEM measurements were carried out in a JEOL 2000 electron
microscope operating at 200 kV.
2B. Plastics. The plastics employed in the present research were the following: polymeric wastes
coming from used greenhouses films of Almeria (Spain), virgin low density polyethylene (LDPE,
(-CH2 - CH2 -)x, Mw = 416,000) and virgin ethylene-vinyl acetate copolymer (EVA, 33 wt % vinyl
acetate content, (-CH2 - CHOCOCH3-)x-(CH2-CH2-)y). Both commercial polymers were provided
by Repsol-YPF. In addition, an homogenous mixture of commercial LDPE (86 wt %) and EVA
copolymer (14 wt %) was prepared by grinding them cryogenically. The plastics were
characterized by Inductively Coupled Plasma spectroscopy (ICP), Thermogravimetric Analyses
(TGA) and Differential Scanning Calorimetry (DSC). ICP measurements were performed with a
VARIAN VISTA AX apparatus. TGA were carried out in a SDT 2960 TA instrument heating the
sample with a rate of 5 ºC min-1 under a 100 Nml min-1 nitrogen flow up to 600 ºC. DSC analyses
were taken using a DSC822e METTLER-TOLEDO device. The sample was heated from –20 to
250ºC with a rate of 10ºC min-1.
2C. Reaction system. Before being loaded into the reactor, the plastic wastes were washed,
dried and ground cryogenically below 1 mm particle size. In addition, the catalysts were also
ground and sieved (mesh size below 75 m). The reaction system used in the thermal and
catalytic cracking experiments is illustrated in Figure 1. It consists of a stainless steel batch
reactor provided with a helicoidal stirrer swept by a continuous nitrogen flow (25 Nml min-1). In a
typical experiment, 10 g of plastic film wastes were introduced into the reactor together with 0.2 g
of the catalyst (plastic / catalyst mass ratio = 50). Thereafter, the reactor is heated up to the
reaction temperature (380 - 420ºC) with a ramp rate of 6ºC min-1 under inert atmosphere, the
glass condenser cooled by an ice trap. The liquid products were separated and weighed whereas
the gaseous products were collected in a gas sampling bag. Gaseous products were analyzed in
a Hewlet Packard 5880 GC equipped with a Porapak Q column. Condensed products were
analyzed in a Varian 3800 GC equipped with a 10 m MXT capillary column. PIONA analyses
(Paraffins, Isoparaffins, Olefins, Naphtenes and Aromatics) were carried out in a Varian 3800 GC
provided with a 100 m length x 0.25 mm i. d. Chrompack capillary column. The conversion was
defined as follows: (mass of collected hydrocarbons Cn, n 40 + mass of acetic acid released)
(mass of loaded film waste)-1 *100. The remaining residue into the reactor after the reaction was
not regarded as product. The mass balances were closed within a 5 % error range.
3. Results and discussion
3A. Plastic film waste characterization. The plastic film waste recovered from Almería
greenhouses (Spain) is mostly made up of both degraded LDPE and EVA copolymer. As a result
of the exposure to the ambient light and air of the film throughout its lifetime (2-3 years), it has
undergone several degradation processes such as oxidation and crosslinking. TGA of the plastic
film waste and both virgin polymers (LDPE and EVA) under inert atmosphere are shown in Figure
2. TGA of the EVA copolymer shows two distinct peaks in the differential curve placed at 340 and
459 ºC, respectively. The former (25 wt %) corresponds to the complete elimination of the vinyl
acetate present in the polymer, that is released as acetic acid whereas the latter (75 wt %) has
been ascribed to the decomposition of the remaining polyethylene-like residue , which agrees
well with the position of the main peak of virgin LDPE degradation (463 ºC). TGA of the film waste
shows one main peak in the differential curve situated at the same temperature (463 ºC) of the
aforementioned, confirming the polyethylenic nature of the film waste. A second small peak
vinyl acetate content of the plastic film waste is roughly 4 wt %. DSC analyses of the plastic film
waste as well as of both virgin polymers (LDPE and EVA) are shown in Figure 3. LDPE exhibits
only one endothermic peak placed at 110ºC corresponding to the polyethylene melting point while
EVA copolymer shows solely a broad one centered at 56ºC with a shoulder at roughly 72ºC. DSC
of the plastic film waste presents a main peak at 110ºC corresponding to the major component of
the refuse, polyethylene. This peak is wider than that of pure LDPE, probably due to the different
degradation processes it has undergone during usage. In addition, a second small peak placed at
57ºC is appreciated that is associated to the small amount of EVA copolymer present in the
The plastic film waste also contains different inorganic fillers usually loaded in its
composition as well as dirt coming from its agriculture usage. ICP analyses of the film waste
indicated the presence of the following elements: Al (0.1 wt %), Ni (0.05 wt %), Ca (0.07 wt %),
Mg (0.05 wt %), K (0.01 wt %), Fe (0.03 wt %) and S (0.17 wt %). According to the TGA
measurements, the total amount of inorganic fillers and dirt, estimated as the final weight above
550 ºC, is quite low (about 1-2 wt %).
3B. Catalyst characterization. The main physicochemical properties of the catalysts used in this
work are shown in Table 1. Al-SBA-15 and Al-MCM-41 are uniform mesoporous aluminosilicates
with pore diameters of 4.7 and 2.0 nm respectively. Al-SBA-15 differ from Al-MCM-41 not only in
pore size but also in both its thicker pore wall (> 3.0 nm) and the presence of certain amount of
micropores (completely absent in Al-MCM-41) . Titanium aluminum Beta (TiAl-Beta) and
nanometer size HZSM-5 (n-HZSM-5) zeolites are crystalline microporous aluminosilicates with a
3D porous structure and a mean pore diameter of 0.63 and 0.55 nm, respectively. n-HZSM-5 has
fully accessible to the bulky polymer macromolecules. Thus, the external surface area of this
material represents almost 20 % of the total surface. All the catalysts have been synthesized with
Si/Al atomic ratios within the 40 - 50 range. Aluminum incorporation into the framework was borne
out by 27Al-MAS-NMR measurements, as the share of tetrahedral aluminum after calcination in all
the catalysts was roughly 90%. The strength of the catalyst acid sites, determined from the
temperature maxima of ammonia programmed desorption (TPD) measurements (see Table 1),
follows the order: n-HZSM-5 > TiAl-Beta > Al-MCM-41 Al-SBA-15.
3C. Catalytic conversion of the plastic film waste. Figure 4 shows the conversions obtained at
420ºC in the cracking of the plastic film waste over the different catalysts as well as that
corresponding to the blank test reaction of thermal degradation. In addition, the results obtained
in both thermal and catalytic cracking of the virgin LDPE at 420ºC have also been included for
establishing a better comparison. As inferred from the figure, the conversion obtained in the
thermal cracking of the film waste is slightly lower than that of the LDPE, despite the release of a
meaningful amount of acetic acid ( 3 wt %) around 350 - 400ºC. This fact suggests that the
plastic film waste is more difficult to be cracked thermally than the commercial LDPE. On the
other hand, catalytic cracking of the plastic film waste over the mesoporous materials (Al-SBA-15
and Al-MCM-41) gave rise to similar or even slightly lower conversions than that of the thermal
cracking. These results are especially striking compared to those obtained in the cracking of the
LDPE since 100 % conversion was attained over both mesoporous catalysts under identical
experimental conditions. In contrast, n-HZSM-5 zeolite was able to degrade completely the film
waste leading to almost 100 % conversion. Consequently, n-HZSM-5 zeolite seems not to be
affected by the plastic film waste composition in contrast with the mesoporous SBA-15 and
Al-MCM-41 catalysts. TiAl-Beta zeolite also shows higher activity (60 %) than thermal cracking and
The selectivity by groups obtained with the catalytic cracking of the plastic film waste over
the different catalysts as well as that corresponding to the blank test reaction at 420ºC are shown
in Figure 5. n-HZSM-5 zeolite shows a remarkable high selectivity towards C1 - C5 hydrocarbons
(60 wt %), the great majority of them being valuable C3 - C5 olefins, whereas both thermal and
catalytic cracking over the other catalysts led to 20 -30 % selectivity towards this hydrocarbon
fraction. The highest selectivity towards C6 - C12 hydrocarbons was obtained over TiAl-Beta
zeolite (> 55 %) and the lowest over n-HZSM-5 zeolite. In addition, both zeolites provided the
lowest amount of heavier C13 - C40 hydrocarbons, unlike the mesoporous catalysts and the
thermal cracking that show selectivities around 30 %. Figure 6 illustrates the selectivity by carbon
atom number obtained in the thermal and catalytic cracking of the plastic film waste over the
different catalysts. n-HZSM-5 zeolite presents a main maximum placed at the C4 hydrocarbon
fraction (28 %), the total selectivity towards the valuable C3 - C5 hydrocarbon fractions being
above 55 %. On the other hand, the product distribution by carbon atom number obtained over
both Al-SBA-15 and Al-MCM-41 catalysts is quite similar to that corresponding to the thermal
PIONA analyses of the C6 - C12 hydrocarbon fraction are shown in Figure 7. Cracking
over Al-MCM-41 and Al-SBA-15 point out the presence of a high and similar content of 1-olefins
and n-paraffins, which are the main products expected from a radical cracking mechanism of the
polyethylene backbone, typical of the thermal degradation . Both activity and selectivity data
indicate that, in the cases of Al-SBA-15 and Al-MCM-41 catalysts, thermal cracking is the major
responsible for their respective product distribution. In contrast, the selectivity results obtained
over both zeolites (TiAl-Beta and n-HZSM-5) are more in line with those reported in the
taking place [24,25]. Selectivity data can be explained in terms of the respective acid strength,
external surface and microporous structure of the zeolites. In the case of n-HZSM-5 zeolite, and
due to its small micropore size ( 0.55 nm), the initial cracking steps mainly proceeds on the
strong acid sites present over its large external surface (82 m2 g-1), giving rise to the primary
cracking products (C3 - C5 olefins) through a carbocationic end-chain cracking mechanism.
Instead, TiAl-Beta zeolite leads mostly to C6 - C12 hydrocarbons due to its both lower acid
strength and external surface as well as slightly higher micropore size (0.63 nm). In this case,
less intense cracking reactions occur whereas secondary C3 - C5 olefin oligomerization reactions
takes place inside the micropores leading to higher hydrocarbons.
The performance of both n-HZSM-5 and TiAl-Beta zeolite for the cracking of the plastic
film waste within the 380-420ºC temperature range is shown in Figure 8. n-HZSM-5 zeolite was
always the most active catalyst regardless of the studied temperature. In addition, it gave rise to a
meaningful cracking conversion (15%) even at a temperature as low as 380ºC and despite the
low amount of used catalyst (under these conditions, the conversion of the thermal cracking
reaction was roughly 3 %). By contrast, at this same temperature, TiAl-Beta zeolite provides
practically the same activity of the bottom thermal cracking reaction.
On the other hand, in order to check the deactivation of n-HZSM-5 zeolite, its activity
evolution with the time was followed at 380ºC, showing conversions of 14, 26 and 39 wt % after
2, 4 and 6 h of reaction, respectively. Hence, its cracking performance proceeds with practically
no decay in activity with the time. In addition, the obtained products at 380ºC are also valuable C2
In a previous work , the presence of EVA copolymer in a virgin LDPE / EVA
copolymer mixture (86/14 w/w) with a vinyl acetate content ( 4%) similar to that of the film waste
here studied, was observed to be detrimental for the cracking over mesoporous catalysts
(Al-MCM-41, Al-SBA-15). This behaviour has been ascribed to the occurrence of crosslinking
reactions after the release of acetic acid, leading to the catalyst deactivation by coke fouling on
the unhindered mesoporous structure of both Al-SBA-15 and Al-MCM-41. A similar phenomenon
may also occur in the cracking of the film waste explaining the low activity of the mesoporous
catalysts. In addition, the medium acid strength of these materials is not probably high enough for
promoting the cracking of the refuse. By contrast, the observed remarkable performance of
n-HZSM-5 can be mostly ascribed to both its great content of strong and accessible external acid
sites, and high resistance to coke deactivation.
The results reported in this work prove that the direct catalytic cracking of a real plastic
film waste is a feasible feedstock recycling procedure provided that a suitable catalyst is used.
Mesoporous solids (Al-MCM-41 and Al-SBA-15), that had shown remarkable performance in the
cracking of the raw low-density polyethylene (LDPE), were practically inactive with the plastic film
waste, probably due to its medium acid strength along with a deactivation phenomenon caused
by the presence of EVA copolymer in the raw refuse. However, n-HZSM-5 zeolite was able to
degrade completely the film waste using a very small amount of catalyst (plastic / catalyst mass
ratio of 50). In addition, more than 55 wt % of C3 - C5 hydrocarbons were obtained over this
catalyst at 420ºC, the majority of them being valuable olefins. Consequently, n-HZSM-5 zeolite
shows remarkable properties for the cracking of plastic film wastes, being capable of surpassing
The authors want to thank “Consejeria de Educación de la Comunidad de Madrid”
(Strategic Group Project) and "Ministerio de Ciencia y Tecnología" (project REN2002-03530 /
TECNO) for their financial support to this research. We are also grateful to REPSOL-YPF for
Association of Plastics Manufacturers in Europe (APME), Summary Report: An analysis of
plastics consumption and recovery in Western Europe 2000, (2002).
J. Aguado, D. P. Serrano, Feedstock Recycling of Plastic Wastes, Royal Society of Chemistry,
 S. Babinchak, CHEMTECH 21(12) (1991) 728.
 G. L. Nelson, CHEMTECH25(12) (1995) 50.
 M. R. Kahn, C. C. Albert, S. J. De Canio, WO Patent 9903 (1995).
 H. K. Mucha, U. Drost, R´02 6th World Congress on Integrated Resources Management,
 H. P. Wenning, J. Anal. Appl. Pyrolysis 25 (1993) 301.
 J. Kim, W. Kaminsky, B. J. Schlesselmann, J. Anal. Appl. Pyrolysis 40-41 (1997) 365.
 Plastic Waste Management Institute Newsletter (Japan), Liquefaction Technology 15(3) (1998)
 A. Corma, S. Cardona, Appl. Catal. B 25 (2000) 151.
 G. Manos, I. Y. Yusof, N. Papayannakos, N. H. Gangas, Ind. Eng. Chem. Res. 40 (2001)
 W. Kaminsky, J. Kim, J. Anal. Appl. Pyrolysis 51 (1999) 127.
 A. R. Songip, T. Masuda, H. Kuwahara, K. Hashimoto, Appl. Catal. B 2 (1993) 153.
 D. P. Serrano, J. Aguado, J. M. Escola, Ind. Eng. Chem. Res.39 (2000) 1177.
 S. Ali, A. A. Garforth, D. H. Harris, D. J. Rawlence, Y. Uemichi, Catal. Today 75 (2002) 247.
 R. Bagri, P. T. Williams, J. Anal. Appl. Pyrolysis63 (2002) 29.
 R. Van Grieken, J. L. Sotelo, J. M. Menéndez, J. A.. Melero, Microporous Mesoporous Mater.
 D. P. Serrano, M. A. Uguina, G. Ovejero, R. Van Grieken, M. Camacho, J. A. Melero, J.
Mater. Chem. 9 (1999) 2899.
 J. Aguado, D. P. Serrano, R. Van Grieken, J. M. Escola, E. Garagorri, Stud. Surf. Sci. Catal.
135 (2001) 273.
 A. Marcilla, A. Gómez, J. A. Reyes-Labarta, Polymer 42 (2001) 8103.
 K. Miyazawa, S. Inagaki, Chem. Commun. (2000) 2121.
 T. P. Wampler, J. Anal. Appl. Pyrolysis, 15 (1989) 187.
 J. Aguado, J. L. Sotelo, D. P. Serrano, J. A. Calles, J. M. Escola, Energy Fuels 11 (1997)
 Bohdan W. Wojciechowski, Ind. Eng. Chem. Res. 36 (1997) 3323.
 A. Corma, Chem. Rev. 95(3) (1995) 475.
 D. P. Serrano, J. Aguado, J. M. Escola, J. M. Rodríguez, L. Morselli, R. Orsi, J. Anal. Appl.
Pyrolysis 68-69 (2003) 481.
Table 1. Physicochemical properties of the catalysts
BET surface area (m2 g-1)
External surface area (m2 g-1)a
Pore Volume (cm3 g-1)b
Pore Diameter (nm)
Crystal size (nm)
Acidity (mmol g-1)c
Al-SBA-15 49 623 - 0.65 4.70 - 242 0.260
Al-MCM-41 40 1240 - 0.83 2.10 - 254 0.254
TiAl-Beta 41 653 22 0.25 0.63 230 329 0.276
n-HZSM-5 45 428 82 0.16 0.55 60 357 0.324
Figure 1. Scheme of the experimental cracking installation.
Figure 2. TGA under inert atmosphere of the plastic samples.
Figure 3. DSC analyses of the plastic samples.
Figure 4. Conversions obtained with the thermal and catalytic cracking of both plastic film waste
and virgin LDPE (T = 420ºC; t = 2 h).
Figure 5. Selectivity by groups obtained with the thermal and catalytic cracking of the plastic film
waste (T = 420ºC; t = 2 h).
Figure 6. Selectivity by carbon atom number obtained with the thermal and catalytic cracking of
the plastic film waste (T = 420ºC; t = 2 h).
Figure 7. PIONA analyses of the C6 - C12 hydrocarbon fraction obtained in the thermal and
catalytic cracking of the plastic film waste at 420ºC.
Figure 8. Evolution with the temperature of the cracking conversion of the plastic film waste over
100 200 300 400 500
0 20 40 60 80 100
100 200 300 400 500
0 20 40 60 80 100
100 200 300 400 500 600
0 50 100 150 200 250
72ºC 56ºC 57ºC
0 20 40 60 80 100
C1 - C5 C6 - C12 C13 - C40
0 20 40 60 80 100
5 10 15 20 25 30 35
0 10 20 30
5 10 15 20 25 30 35
0 10 20 30
5 10 15 20 25 30 35
0 10 20 30
5 10 15 20 25 30 35
0 10 20 30
0 5 10 15 20 25 30 35
0 10 20 30 n-HZSM-5 TiAl-Beta Al-SBA-15 Al-MCM-41
CARBON ATOM NUMBER
0 10 20 30 40 50 60
Al-SBA-15 Al-MCM-41 TiAl-Beta n-HZSM-5
380 400 420
0 20 40 60 80 100